i n t e r n a t i o n a l j o u r n a l o f h y d r o g e n e n e r g y 4 5 ( 2 0 2 0 ) 1 3 6 8 3 e1 3 6 9 2 Available online at www.sciencedirect.com ScienceDirect journal homepage: www.elsevier.com/locate/he Electrodes modified with Ni electrodeposition decrease hexavalent chromium generation in an alkaline electrolysis process Froylan Alonso Soriano Moranchell a, Juan Manuel Sandoval Pineda a, ndez Perez b, Usiel Sandino Silva-Rivera a, Jesús Nahúm Herna lez Huerta b,* Claudia Alicia Cortes Escobedo c, Rosa de Guadalupe Gonza Instituto Politecnico Nacional-ESIME-Azc, SEPI, Av. De las Granjas, No. 682, Azcapotzalco, CP 02250, CDMX, Mexico b Instituto Politecnico Nacional -ESIQIE, Laboratorio de Investigacion de Electroquı́mica, UPALM, CP 07738, CDMX, Mexico c Instituto Politecnico Nacional-CIITEC, Cda. Cecati s/n, Col. Sta. Catarina, Azcapotzalco, CP 02250, CDMX, Mexico a highlights One of the challenges to widespread use of water electrolysis is to reduce maintenance time. Cr6þwas detected out of norm in electrolyte using stainless steel electrodes. Cr6þ is very dangerous metal ion, generates different types of cancer in people. In modified Ni electrodes, Cr6þ was detected within norm in the electrolyte. Electrode materials must be stable at high anodic potential and alkaline media. article info abstract Article history: Alkaline water electrolysis is one of the easiest methods used to produce hydrogen, of- Received 21 July 2019 fering the advantages of simplicity and low cost. The challenges for the widespread use of Received in revised form water electrolysis are to reduce energy consumption, cost and maintenance and to in- 9 December 2019 crease the reliability, durability and safety of the process. The alkaline electrolysis of water Accepted 6 January 2020 has been used for many years to obtain H2 and O2; however, less expensive, more active, Available online 31 January 2020 endurable and efficient electrodes must be designed. Stainless steel (SS) is considered one of the least expensive electrode materials for alkaline electrolysers, since it is relatively Keywords: chemically stable and has a low overpotential. Nevertheless, SS anodes do not withstand Alkaline electrolyser high concentration alkaline solutions because they undergo a corrosion process. If the Hydrogen electrolyser operates at a voltage of up to 1.6 V, it can generate Fe3O4 and hazardous Hexavalent chromium hexavalent chromium (Cr6þ) at the anode. Hexavalent chromium is generated when the Modified electrodes chromium-containing stainless steel electrodes undergo an electro-oxidation process. In Ni-electrodeposited electrode this work, a low power alkaline electrolyser was designed. In the first step, six electrodes were manufactured of stainless steel. In the second step, a nickel layer with matte or opaque finish was deposited on the SS surfaces to improve their resistance to corrosion and wear. Then, the performance curves and the production of hexavalent chromium were determined. The performance curve after 70 h of operation with nickel-plated electrodes showed an overpotential of 0.5 V at 10 A compared with stainless steel electrodes. Cr6þ was * Corresponding author. lez Huerta). E-mail address: [email protected] (R.G. Gonza https://doi.org/10.1016/j.ijhydene.2020.01.050 0360-3199/© 2020 Hydrogen Energy Publications LLC. Published by Elsevier Ltd. All rights reserved. 13684 i n t e r n a t i o n a l j o u r n a l o f h y d r o g e n e n e r g y 4 5 ( 2 0 2 0 ) 1 3 6 8 3 e1 3 6 9 2 detected in the electrolyte and bubbler water of the system using SS electrodes at values that exceeded the standard (>0.5e1 mg L1). If the electrolyser used Ni-electrodeposited electrodes, Cr6þ was observed in quantities within the normal range (<0.1 mg L1). It is very important to prepare modified anodes with nickel electro-deposited, this process prevents the generation of hexavalent chromium, contamination of the electrolyte and reduces maintenance times. The above compensates the slight increase in electrodes cost and energy consumed by the electrolyser. © 2020 Hydrogen Energy Publications LLC. Published by Elsevier Ltd. All rights reserved. Introduction Alkaline water electrolysis is an inexpensive method for hydrogen production, offering the advantage of simplicity. The challenges preventing the widespread use of water electrolysis are to reduce its energy consumption, cost and maintenance and to increase its reliability, durability and safety. Alkaline electrolysis in water has been used for many years to generate H2 and O2. However, less expensive, more active and robust cathodic and anodic electrodes must be designed. Water electrolysis comprises two reactions: a hydrogen evolution reaction (HER) at the cathode and an oxygen evolution reaction (OER) at the anode. Both reactions must have a low overpotential to increase the efficiency. The overvoltage of the OER has been identified as the greatest source of energy loss in water electrolysis. In addition, the anode can undergo electrocorrosion processes, resulting in higher overpotentials and shorter lifetimes . This overpotential is directly related to the potential difference necessary to drive the system at a higher current density, and therefore, is directly related to the cost of the hydrogen production, as an alkaline electrolyser can operate at 0.2e0.4 A cm2 . Stainless steel is considered one of less expensive electrode materials used for alkaline electrolysers. Stainless steel (304 and 316) is composed of 18e22% w of Cr, 8e11% Ni and 2% Mo. Stainless steel is chemically stable in alkaline medium, but when a potential >1.6 V is applied between electrodes, corrosion processes occur at the anode. A low potential (1.6 V) must be applied to minimize this corrosion process, but the typical voltage normally ranges from 1.8 to 2.4 V for the monopolar configuration of an electrolysis system . Articles analyzing the corrosion processes and determining the compounds generated during operation of a low power alkaline electrolyser were not identified in a literature search. Some electrolyser designs have been discussed in the literature. For example, Lavorante MJ et al.  evaluated the performance of four different kinds of stainless steel 316L mechanized electrodes, which were used in alkaline water electrolysers for hydrogen production. El-Kassaby MM et al.  constructed a simple and innovative HHO generation system using stainless steel plates as the electrodes, and the optimized parameters were the number of neutral plates, the distance between the plates and the electrolyte type (NaOH or rez-Alonso FJ et al.  prepared Ni/Fe electrodes by KOH). Pe electrodeposition on different substrates; the OER overpotential appeared to be lower for the electrodes with higher Ni concentrations, as the Ni75Fe25-Nf electrode exhibited the better configuration to obtain the lowest overpotentials (2.1 V) and displayed high stability as the anode after 70 h of operation in water alkaline electrolysis. Hammoudi M et al.  presented a multiphysics model used for the design and diagnosis of the alkaline electrolysers. Sandeep KC et al.  postulated that commercial hydrogen production by water electrolysis is limited by the high cost of electricity. In that study, porous nickel electrodes were manufactured manually on a laboratory scale. Ziems C et al.  developed two pressurized alkaline electrolyser prototypes that were built to investigate the effects of different temperatures and pressures. Khalilnejad A et al.  designed a small alkaline electrolyser with a 25% alkaline (KOH) solution and maximum power of 60 W, and they integrated a hybrid windphotovoltaic hydrogen system. Amores E et al.  designed new advanced alkaline electrolysers that were integrated with renewable energy sources. Other studies have also described electrolyser designs [12e14] and dual combustion, hydrocarbon-hydrogen, in an internal combustion engine [15e23]. Nickel is considered the most suitable material for alkaline electrolysers, since it is highly chemically stable, relatively inexpensive and can be used as a catalytic material for cathodic and anodic reactions. The methods used to prepare electrodes are important factors in terms of the effects on the electrode surface properties, such as roughness and stability. One of the methods used for metal deposition over metallic substrates is electrodeposition. Material selection and electrode modifications in the cell design are important in water electrolysis. Many studies have examined Ni and Ni alloy electrodes in alkaline medium [1,24e35]. In this work, an alkaline electrolyser was designed. In the first step, six electrodes were manufactured of stainless steel. Nickel with a matte or dull finish was deposited on stainless steel surfaces in the second step to improve corrosion and wear resistance. The electrolyser performance curve and production of hexavalent chromium (Cr6þ) were determined after 70 h of operation. Materials and methods Preparation of modified electrodes Stainless steel 304 gauge 20 was used as the substrate material for the electrodes (anodes and cathodes). Nickel with a matte or dull finish was deposited on the stainless steel surfaces to i n t e r n a t i o n a l j o u r n a l o f h y d r o g e n e n e r g y 4 5 ( 2 0 2 0 ) 1 3 6 8 3 e1 3 6 9 2 improve corrosion and wear resistance. The electrodeposition method is an electrochemical technique, in which a thin layer of metallic nickel is deposited on a substrate based on Faraday's laws. The process of electrodeposition on stainless steel consists of three steps, each involving a specific solution that requires an electrochemical system, namely: a) Cleaning: This process includes the polishing of the base metal and anodic electrolytic cleaning (AEC) of the electrodes to eliminate dust, grease and particles remaining on the surface. In AEC, the anode is the working electrode and is placed in an alkaline electrolyte solution (3% w), and the electrolysis of water occurs at 5e7 A dm2. The oxygen formed in the reaction cleans the surface by removing dirt. b) Surface pretreatment (SP): A high degree of adhesion between the deposit and the substrate is critical in all electrodeposited applications. In this case, the adhesion of nickel onto the stainless steel support becomes a very difficult task, and a surface pretreatment is necessary before nickel deposition. Good adhesion of nickel on a stainless steel surface is achieved through an electrochemical pretreatment with solution composed of NiCl2 (240 g L1) and HCl (120 ml L1). In SP, the cathode is the working electrode and is placed in an acid electrolyte solution, and the electrolysis of water occurs at 2.5 V. The hydrogen formed in the reaction produces an electrolytic pickling on the electrode surface. c) Deposit nickel: The present study used the Watts method for nickel electrodeposition. An electrodeposition bath was prepared by mixing 300 g L1 NiSO4*6H2O, 60 g L1 NiCl2*6H2O, and 45 g L1 H3BO3 at 55e60 C, pH 4.5 at 5.4 A dm2 and 20 min with agitation. The components in Watts solutions affect the quality of nickel deposition. Nickel sulfate improves conductivity and metal distribution on the substratum surface and limits the cathode current density for generating sound nickel deposits. Nickel chloride improves anode corrosion, increases the conductivity and uniformity of the coating thickness distribution and helps to refine the grain size and minimize formation of nodules. Boric acid is added for buffering purposes and affects the appearance of the deposits. Deposits may be cracked and burned at low boric acid concentrations . Corrosion protection in real applications mainly depends on the thickness of the nickel layer. The thickness that should be applied depends on the specific application. For example, the thickness of the nickel layer in optical and electronic applications may be 5 mm. The thickness may be 7 mm to protect the product purity, such as ferrous containers. Nickel coatings on automotive components, such as hydraulic rams, cylinder liners, and shock absorbers, may be 125 mm thick to provide corrosion and wear resistance. Equation (1) was used to calculate the thickness of the nickel layer, s in micrometers (mm): s¼ m*1 105 1:095 105 *I*t*h 0:123 105 *I*t*h ¼ ¼ 8:907*A A d*A (1) where m (g) is the amount of nickel deposited at the cathode (or dissolved at the anode), d (8.907 g cm3) is the density of nickel, A (cm2) is the electrode area, 1 105 is the conversion 13685 factor from cm to mm, I (A) is the electric current that flows through the plating tank, t (h) is the time that the current flows, and h is the current efficiency ratio (95%). The proportionality constant 1.095 in g/Ah equals М/nF, where М is the atomic weight of nickel (58.69 gr mol1), n is the number of electrons in the electrochemical reaction (2), and F is Faraday's constant, which is equal to 26.799 A-h (more commonly listed as 96,500 C). Physical characterization Scanning electron microscopy (SEM) was used to determine surface morphology of the nickel plating using a Sirion FEGSEM microscope from FEI. X-ray diffraction (XRD) patterns were recorded to analyze the surface of stainless steel and nickel-plated electrodes after 70 h of operation using a Bruker D2 Phaser. The diffraction parameters were the diffraction angle 2q that ranged from 20 to 80 . Cu Ka radiation (l ¼ 1.5418 A) was used in all experiments. Design of the electrolyser and performance curves The electrolyser system was designed to support at a power of up to 100 W. The following parameters related to the performance must be identified to evaluate the electrolysis system: (a) cell monopolar configurations, parallel connection of the electrodes, (b) electrode gap of 2.3 mm and (c) operating conditions: voltage ranging from 1.5 V to 6 V, applied current ranging from 0.1 A to 10 A, temperature of 60 C, electrolyte concentration (5% w NaOH solution, deionized water was used). In the first stage, 6 stainless steel (304-19 gauge) electrodes (3 anodes and 3 cathodes, each with an area of 74 cm2) were in contact with a 5% w alkaline solution (NaOH); this concentration was chosen to avoid the corrosive effects of NaOH and increase the simplicity of the gas purification system. In the second stage, the electrodes were modified by electrodepositing Ni onto the stainless steel substrates. Fig. 1 shows the CAD diagram of the electrolyser. The performance curves were obtained using a test system that included a power source, phase separator or electrolyte recirculator, bubbler, dryer, mass flow meter and electrolyser, as shown in Fig. 2. A controlled current was applied from 0.1 to 10 A. The oxyhydrogen gas production was measured with an ALICAT flowmeter. By definition, a water electrolysis system always produces hydrogen at twice the volume of oxygen (mixture of hydrogen and oxygen is called oxyhydrogen gas). The electrolyser was operated for 70 h (at 10 A), and performance curves were obtained every 10 h. The amount of hexavalent chromium (Cr6þ) dissolved in the electrolyte and water bubbler was determined with a photometric technique using 1,5-diphenylcarbazide. The spectrophotometer (UV/VIS) is an instrument that measures the absorption of light. Cr6þ oxidizes 1,5-diphenylcarbazide to 1,5-diphenylcarbazone, which forms a violet-colored complex with the Cr3þ product. At 550 nm, the extinction of the dye displays a linear relationship with the Cr6þ concentration. The evaluation was performed using the calibration function and a reference solution. 13686 i n t e r n a t i o n a l j o u r n a l o f h y d r o g e n e n e r g y 4 5 ( 2 0 2 0 ) 1 3 6 8 3 e1 3 6 9 2 Fig. 1 e CAD diagram of the alkaline electrolyser. Fig. 2 e Diagram of the electrolyser test system. Results and discussion Performance electrolyser Fig. 3 shows the stacked experimental arrangement of the electrolyser. Importantly, the electrolyser must be tested in a ventilated area without flammable materials (solvents, paper, etc.). The gas produced must be bubbled in distilled water and passed through a desiccant to remove electrolyte drag. Finally, the system must have an external hydrogen vent to avoid hydrogen accumulation in the work area. Fig. 4(aeb) shows the performance curve of the alkaline electrolyser (EA) stack. In the initial test with stainless steel electrodes (SSE), the electrolyser required a lower voltage (4.1 V) at 10 A than nickel-electrodeposited electrodes (NiEE) (4.4 V). The performance curves were obtained every 10 h and show a decrease in the potential demand. Although no definite trend for the required voltage was observed with respect to the operating time, this lack of a trend was attributed to the superficial changes and corrosion processes of the electrodes, which will be analyzed in the next section. Fig. 3 e Stacked alkaline electrolyser. i n t e r n a t i o n a l j o u r n a l o f h y d r o g e n e n e r g y 4 5 ( 2 0 2 0 ) 1 3 6 8 3 e1 3 6 9 2 13687 Fig. 4 e Electrolyser performance curves: a) SSE (stainless steel electrodes) and b) NiEE (nickel electrodeposited electrodes). Fig. 5 shows the performance of electrolyser after 70 h of operation, and the voltage of the stainless steel electrodes was lower than the electrolyser with nickel-electrodeposited electrodes at 10 A. The voltage required by NiEE was higher because the nickel electrodeposited with matte finishes had a lower conductivity than that of stainless steel. According to Shreir LL. et al. , nickel decomposes particularly slowly in alkaline medium because it forms a passive layer. The mechanism of film formation is complex, involving the adsorption of OH ions to form a prepassive layer followed by dissolution, and may proceed in three consecutive steps as follows : Ni þ OH/NiOHadsorber þ e þ NiOHadsorber / NiOH þ e þ 2þ NiOH / Ni þ OH (2) brown layer is iron oxide (Fe2O3); therefore, if stainless steel is used as an anode in alkaline media, metallic iron is oxidized. Fig. 7(a) shows an image of the stainless steel cathode after 70 h of operation. The electrode surface is covered by a dark layer, which was analyzed using the XRD technique. The diffractogram is shown in Fig. 7(b), and the dark layer is tetrataenite (intermetallic alloy of Fe0.5O7Ni0.49); therefore, if stainless steel is used as an anode in alkaline media, iron and nickel are leached or dissolved (with different oxidation states: Ni2þ, Fe2þ, Fe3þ, etc.) and some ions are deposited on the cathode. Fig. 8(a) shows an image of the nickel-electrodeposited electrode, and Fig. 8(bec) show SEM images, both of which were captured before the operation of the electrolyser. Electrodeposition was homogeneous with a granular morphology, (3) (4) The following reactions are responsible for the transition from active to passive behavior: NiOHadsorber þ OH / NiðOHÞ2Y þ e (5) NiðOHÞ2Y / NiOY þ H2 O (6) The formation of a passive layer and Ni dissolution result from the competition among these reactions. The ratedetermining step changes (from 4 to 3 to 2) as the overvoltage is increased. At potentials where reactions 4 and 5 are possible, the percentage of the surface area covered with an oxide film increases, and accordingly, the current density gradually decreases in the transition region. Electrode analysis An image of the stainless steel anode captured after 70 h of operation is shown in Fig. 6(a). A brown layer is observed on surface of the electrode, which was analyzed using the XRD technique. The diffractogram is shown in Fig. 6(b), and the Fig. 5 e Electrolyser performance: initial results and results obtained after 70 h of operation with SSE and NiEE. 13688 i n t e r n a t i o n a l j o u r n a l o f h y d r o g e n e n e r g y 4 5 ( 2 0 2 0 ) 1 3 6 8 3 e1 3 6 9 2 Fig. 6 e Stainless steel electrode after 70 h of operation: a) image of the anode and b) diffractogram. Fig. 7 e Stainless steel electrode after 70 h of operation: a) image of the cathode and b) tetrataenite diffractogram. and the composition is shown in Fig. 8(d), which indicated 100% nickel metal. Fig. 9 shows images of the nickel-plated electrodes (cathode and anode) after 70 h of operation. The electrode surface of the anode shows a grayish layer in Fig. 9(a), which was analyzed using the XRD technique. The diffractogram shows Ni(OH)2 in Fig. 9(b), which is consistent with the findings reported by Bari et al.  and is described in equations (2)e(5). However, Fe2O3 is observed is less frequently than SSE. The electrode surface of cathode shows a gray layer in Fig. 9(d), which was analyzed using the XRD technique. The diffractogram shows Ni and NiO in Fig. 9(e), consistent with the results reported in the literature. The SEM images in Fig. 9(c) and (f) show a homogeneous surface, without the original granular morphology. This analysis indicates a change in the surface morphology and composition of both electrodes. Electrolyte analysis When SSEs were used, iron leached or dissolved from the anode to form a brown precipitate in the electrolyte, as shown Fig. 10(a). Fe2O3 was produced according to the XRD data shown in Fig. 6(b). The electrolyte showed a yellowish color, which was attributed to the generation of hexavalent chromium (Cr6þ) when the chromium-containing stainless steel electrodes undergo an electro-oxidation process. When NiEEs were used, the electrolyte was clear and contained white precipitates (NiO, according to Refs. [3,37]), as shown in Fig. 10(b). Therefore, the electrolyte was analyzed with UVevis spectroscopy to determine the amount of chromium dissolved in the electrolyte and bubbler water. Hexavalent chromium (Cr6þ) is listed as compound number 16 in the Agency for Toxic Substances and Disease Registry, Priority List of Hazardous Substances (ATSDR, 1999) . The solutions were analyzed after 70 h of operation. First, two 100 mL samples of bubbler water and electrolyte from the recirculator vessel were collected from both systems using SSEs and NiEEs. The Mexican regulation (NOM-002SEMARNAT-1996) indicates that 1 mg L1 of Cr6þ is the instantaneous maximum limit, and 0.5 mg L1 is the maximum weekly average limit . Table 1 shows the Cr6þ concentrations in the samples. i n t e r n a t i o n a l j o u r n a l o f h y d r o g e n e n e r g y 4 5 ( 2 0 2 0 ) 1 3 6 8 3 e1 3 6 9 2 13689 Fig. 8 e Nickel electrodeposited electrode before the operation of the electrolyser: a) image of the cathode or anode, b) SEM image at 60 mm, c) SEM image at 10 mm, d) spectrum showing the composition of the electrodeposited Ni. As shown in Table 1, SSE formed Cr6þ at levels that exceeded the regulation in the recirculator vessel and bubbler water. This metal ion is very dangerous, and a chemical treatment is necessary to eliminate Cr6þ. In addition, if the electrolyser used NiEEs, Cr6þ was detected in quantities between the normal levels in both samples from the recirculator vessel and bubbler water. Thus, the nickel-electrodeposited electrode generates much less Cr6þ. The generation of ions (Cr6þ and Fe2O3) is attributed to defects in nickel electrodeposition, which will be reviewed and reported in future studies. Electrode materials should be stable and should not corrode in the operating alkaline media (pH 10e14) at the required voltages (1.5e5 V) and at intermediate temperatures Fig. 9 e Ni electrodeposited electrodes after 70 h of operation a) Image of the anode, b) anode diffractogram, c) SEM image of the anode, d) image of the cathode, e) cathode diffractogram, and f) SEM image of the cathode. 13690 i n t e r n a t i o n a l j o u r n a l o f h y d r o g e n e n e r g y 4 5 ( 2 0 2 0 ) 1 3 6 8 3 e1 3 6 9 2 Fig. 10 e a) Electrolyte with SSE and, b) electrolyte with NiEE. Table 1 e Cr6þ concentrations in the samples. Electrolyser 1(SSE) 1 (SSE) 2 (NiEE) 2 (NiEE) Sample source Sample Cr6þ(mg L1) Recirculator Bubbler Recirculator Bubbler 1 2 3 4 1.766 0.800 0.077 0.019 (30e60 C). The following compounds formed when the various electrodes were used: Anode Cr6þ þ Fe2 O3 Stainless steel electrode ! CrO2 4 10 A; 60 C (7) Cathode Stainless steel electrode ! Fe0:5 O7 Ni0:49 10 A; 60 C (8) Anode Ni electrodeposited electrode ! NiðOHÞ2 þ Fe2 O3 10 A; 60 C (9) Cathode Ni electrodeposited electrodes ! Ni þ NiO 10 A; 60 C showed an overpotential of 0.5 V at 10 A. Compared with stainless steel electrodes, the required voltage is higher for NiEEs because the nickel electrodeposited with matte finishes had a lower conductivity than the stainless steel. The SEM and XRD analyses indicate a change in the surface morphology and composition of both electrodes after the electrolysis process. With stainless steel electrodes (SSE) Hexavalent chromium was detected in the electrolyte and bubbler water of the system using stainless steel electrodes (SSE) that exceeded the standard (>0.5e1 mg L1). When nickel-plated electrodes (NiEE) were used, the Cr6þ concentration was observed in quantities near the normative value. It is very important to prepare modified anodes with nickel electrodeposited, this process prevents the generation of hexavalent chromium, contamination of the electrolyte and reduces maintenance times. The above compensates the slight increase in electrodes cost and energy consumed by the electrolyser. This study is expected to serve as a reference for the proper design of low power alkaline electrolysers, and stable and nonhazardous materials should always be used to construct the electrodes. (10) It is very important to prepare modified anodes with nickel electro-deposited, this process prevents the generation of hexavalent chromium, contamination of the electrolyte and reduces maintenance times. The above compensates the increase in electrodes cost and energy consumed by the electrolyser. Acknowledgements The authors acknowledge the financial support from IPN multidisciplinary project SIP-2024 (2019e2020) and CONACYT: CEMIE-Ocean project 249795: Transversal Line I-LT1 and Basic Science Project A1-S-15770. The authors acknowledge Dra. Mabel Vaca Mier from UAM-Azc for the support of the hexavalent chromium determination. Conclusions The challenges that must be overcome prior to the widespread use of water electrolysis are to reduce the energy consumption, cost and maintenance and to increase the reliability, durability and safety of the process. The performance curve generated after 70 h of operation with nickel-plated electrodes references ttir CK, Nielsen LP, Møller P. Development of  Kjartansdo durable and efficient electrodes for large-scale alkaline water i n t e r n a t i o n a l j o u r n a l o f h y d r o g e n e n e r g y 4 5 ( 2 0 2 0 ) 1 3 6 8 3 e1 3 6 9 2                electrolysis. Int J Hydrogen Energy 2013;38:8221e31. https:// doi.org/10.1016/j.ijhydene.2013.04.101. Ge X, Sumboja A, Wuu D, An T, Li B, Goh F, Hor T, Zong Y, Liu Z. ACS Catal 2015;5:4643e67. https://doi.org/10.1021/ acscatal.5b00524. Shreir LL, Jarman RA, Burstein GT. In: Metal/environment reaction, corrosion. 3rd ed., vol 1. London, UK: Newnese Butterworths; 2000. reprinted 2000. Lavorante MJ, Franco JI. Performance of stainless steel 316L electrodes with modified surface to be use in alkaline water electrolyzers. Int J Hydrogen Energy 2016;41:9731e7. https:// doi.org/10.1016/j.ijhydene.2016.02.096. EL-Kassaby MM, Eldrainy YA, Khidr ME, Khidr KI. Effect of hydroxy (HHO) gas addition on gasoline engine performance and emissions. Alexandria Eng J 2016;55:243e51. https:// doi.org/10.1016/j.aej.2015.10.016. rez-Alonso FJ, Ada n C, Rojas S, Pen ~ a MA, Fierro JLG. Ni/Fe Pe electrodes prepared by electrodeposition method over different substrates for oxygen evolution reaction in alkaline medium. Int J Hydrogen Energy 2014;39:5204e12. https:// doi.org/10.1016/j.ijhydene.2013.12.186. Y, Doumbia ML. Hammoudi M, Henao C, Agbossou K, Dube New multi-physics approach for modelling and design of alkaline electrolyzers. Int J Hydrogen Energy 2012;37:13895e913. https://doi.org/10.1016/ j.ijhydene.2012.07.015. Sandeep KC, Kamath S, Mistry K, Kumar AM, Bhattacharya SK, Bhanja K, Mohan S. Experimental studies and modeling of advanced alkaline water electrolyser with porous nickel electrodes for hydrogen production. Int J Hydrogen Energy 2017;42:12094e103. https://doi.org/10.1016/ j.ijhydene.2017.03.154. Ziems Ch, Tannert D, Joachim H, Krautz A. Project presentation: design and installation of advanced high pressure alkaline electrolyzer-prototypes. Energy Procedia 2012;29:744e53. https://doi.org/10.1016/ j.egypro.2012.09.087. Khalilnejad A, Riahy GH. A hybrid wind-PV system performance investigation for the purpose of maximum hydrogen production and storage using advanced alkaline electrolyzer. Energy Convers Manag 2014;80:398e406. https:// doi.org/10.1016/j.enconman.2014.01.040. Amores E, Rodrıguez J, Carreras Ch. Influence of operation parameters in the modeling of alkaline water electrolyzers for hydrogen production. Int J Hydrogen Energy 2014;39:13063e78. https://doi.org/10.1016/ j.ijhydene.2014.07.001. Marini S, Salvi P, Nelli P, Pesenti R, Villa A, Berrettoni M, Zangari G, Kiros Y. Advanced alkaline water electrolysis. Electrochem acta 2012;82:384e91. https://doi.org/10.1016/ j.electacta.2012.05.011. Manabe A, Kashiwase M, Hashimoto T, Hayashida T, Kato A, Hirao K, Shimomura I, Nagashima I. Basic study of alkaline water electrolysis. Electrochim Acta 2013;100:249e56. https:// doi.org/10.1016/j.electacta.2012.12.105. ttir C, Allebrod A, Mogensen F, Møller MB, Yde L, Kjartansdo Hilbert P, Dierking A. 2nd generation alkaline electrolysis: final report. Arhus University Business and Social Science e Centre for Energy Technologies; 2013. Horcasitas-Verdiguel M, Sandoval-Pineda JM, Grunstein n-Balaguer LF, Gonza lez-Huerta RG. Design Ramı́rez BA, Tera and manufacture of ICE test module to reduce gasoline consumption using oxyhydrogen gas from an alkaline electrolyzer. ACS Energy Fuel 2016;30:6640e5. https://doi.org/ 10.1021/acs.energyfuels.6b00709. Becerra-Ruiz JD, Gonzalez-Huerta RG, Gracida A, AmaroReyes A, Macias-Bobadilla G. Using green-hydrogen and bioethanol fuels in internal combustion engines to reduce               13691 emissions. Int J Hydrogen Energy 2019;44:12324e32. https:// doi.org/10.1016/j.ijhydene.2019.02.211. Trujillo-Olivares I, Soriano-Moranchel F, Alvarez lez-Huerta RG, Sandoval-Pineda JM. Zapata LA, Gonza Design of alkaline electrolyser for integration in diesel engines to reduce pollutants emission. Int J Hydrogen Energy 2019;44:25277e86. https://doi.org/10.1016/ j.ijhydene.2019.07.256. Ouchikh S, Lounici MS, Tarabet L, Loubar K, Tazerout M. Effect of natural gas enrichment with hydrogen on combustion characteristics of a dual fuel diesel engine. Int J Hydrogen Energy 2019;44:13974e87. https://doi.org/10.1016/ j.ijhydene.2019.03.179. Alper YA. Effects of ignition advance on a dual sequential ignition engine at lean mixture for hydrogen enriched butane usage. Int J Hydrogen Energy 2019;44:15575e86. https://doi.org/10.1016/j.ijhydene.2019.04.088. Tüchler S, Dimitriou P. On the capabilities and limitations of predictive, multi-zone combustion models for hydrogendiesel dual fuel operation. Int J Hydrogen Energy 2019;44:18517e31. https://doi.org/10.1016/ j.ijhydene.2019.05.172. Jabbr AI, Koylu UO. Influence of operating parameters on performance and emissions for a compression-ignition engine fueled by hydrogen/diesel mixtures. Int J Hydrogen Energy 2019;44:13964e73. https://doi.org/10.1016/ j.ijhydene.2019.03.201. Dimitriou P, Tsujimura T, Suzuki Y. Low-load hydrogendiesel dual-fuel engine operation e a combustion efficiency improvement approach. Int J Hydrogen Energy 2019;44:17048e60. https://doi.org/10.1016/ j.ijhydene.2019.04.203. Koten H. Hydrogen effects on the diesel engine performance and emissions. Int J Hydrogen Energy 2018;43:10511e9. https://doi.org/10.1016/j.ijhydene.2018.04.146. Muller ChI, Rauscher T, Schmidt A, Schubert T, Weigarber T, Kieback B, Ronntzsch L. Electrochemical investigations on amorphous Fe-base alloys for alkaline water electrolysis. Int J Hydrogen Energy 2014;3:8926e37. https://doi.org/10.1016/ j.ijhydene.2014.03.151. Jong-Hoon K, Jung-Nam L, Chung-Yul Y, Kyo-Beum L, Woong-Moo L. Low-cost and energy-efficient asymmetric nickel electrode for alkaline water electrolysis. Int J Hydrogen Energy 2015;40:10720e5. https://doi.org/10.1016/ j.ijhydene.2015.07.025. Schalenbach M, Kasian O, Mayrhofer KJJ. An alkaline water electrolyzer with nickel electrodes enables efficient high current density operation. Int J Hydrogen Energy 2018;43:11932e8. https://doi.org/10.1016/ j.ijhydene.2018.04.219. Chanda D, Hnat T, Paidar M, Bouzek K. Evolution of physicochemical and electrocatalytic properties of NiCo2O4 (AB2O4) spinel oxide with the effect of Fe substitution at the A site leading to efficient anodic O2 evolution in an alkaline environment. Int J Hydrogen Energy 2014;39:5713e22. https:// doi.org/10.1016/j.ijhydene.2014.01.141. Kuleshov VN, Kuleshov NV, Grigoriev SA, Udris EY, Millet P, Grigoriev AS. Development and characterization of new nickel coatings for application in alkaline water electrolysis. Int J Hydrogen Energy 2016;41:36e45. https://doi.org/10.1016/ j.ijhydene.2015.10.141. Rauscher T, Muller ChI, Schmidt A, Kieback B, Reontzsch L. Ni-Mo-B alloys as cathode material for alkaline water electrolysis. Int J Hydrogen Energy 2016;41:2165e76. https://doi.org/10.1016/ j.ijhydene.2015.12.132. Gonzalez-Buch C, Herraiz-Cardona I, Ortega EM, Mestre S, Perez-Herranz V. Synthesis and characterization of Au- 13692 i n t e r n a t i o n a l j o u r n a l o f h y d r o g e n e n e r g y 4 5 ( 2 0 2 0 ) 1 3 6 8 3 e1 3 6 9 2 modified macroporous Ni electrocatalysts for alkaline water electrolysis. Int J Hydrogen Energy 2016;41:764e72. https:// doi.org/10.1016/j.ijhydene.2015.10.142.  Solmaz R, Doner A, Dogrubas M, Erdogan IY, Kardas G. Enhancement of electrochemical activity of Raney-type NiZn coatings by modifying with PtRu binary deposits: application for alkaline water electrolysis. Int J Hydrogen Energy 2016;41:1432e40. https://doi.org/10.1016/ j.ijhydene.2015.11.027.  Solmaz R, Salcı A, Yuksel H, Dogrubas M, Kardas G. Preparation and characterization of Pd-modified Raney-type NiZn coatings and their application for alkaline water electrolysis. Int J Hydrogen Energy 2017;42:2464e75. https:// doi.org/10.1016/j.ijhydene.2016.07.221.  Egelund S, Caspersen M, Nikiforov A, Møller P. Manufacturing of a LaNiO3 composite electrode for oxygen evolution in commercial alkaline water electrolysis. Int J Hydrogen Energy 2016;41:10152e60. https://doi.org/10.1016/ j.ijhydene.2016.05.013.  Chanda D, Basu S. Electrochemical synthesis of Li-doped NiFeCo oxides for efficient catalysis of the oxygen evolution reaction in an alkaline environment. Int J Hydrogen Energy 2018;43:21999e2011. https://doi.org/10.1016/ j.ijhydene.2018.10.078.  Koj M, Gimpel T, Schade W, Turek T. Laser structured nickeliron electrodes for oxygen evolution in alkaline water electrolysis. Int J Hydrogen Energy 2019;44:12671e84. https:// doi.org/10.1016/j.ijhydene.2019.01.030.  Jacobs J, Testa SM. Overview of chromium(VI) in the environment: background and history. 2004. L1608_C01.fm.  Di Bari GA. Capı́tulo 3 electrodeposition of nickel. Modern electroplating. EUA: John Wiley & Sons Inc; 2010.  Estados Unidos de America U.S Department Of Health And Human Services. Toxicological profile of chromium. Citado el 24 de junio del 2017 en el sitio web, https://www.atsdr.cdc. gov/toxprofiles/tp7.pdf; 2012.  Estados Unidos Mexicanos. Secretaria de Medio ambiente y recursos naturales. 1998. NOM-002-ECOL-1996.